Optimization of an organic memristor as an adaptive memory element
Tatiana Berzina,1,2Anteo Smerieri,1Marco Bernabò,3Andrea Pucci,3Giacomo Ruggeri,3 Victor Erokhin,1,2,a兲 and M. P. Fontana1,2
Department of Physics, University of Parma, Viale Usberti 7A, Parma 43100, Italy 2
CRS SOFT CNR-INFM, Rome 00185, Italy
3Department of Chemistry and Industrial Chemistry, University of Pisa, Via Risorgimento 35, Pisa 56126, Italy
共Received 9 April 2009; accepted 14 May 2009; published online 24 June 2009兲
The combination of memory and signal handling characteristics of a memristor makes it a promising candidate for adaptive bioinspired information processing systems. This poses stringent requirements on the basic device, such as stability and reproducibility over a large number of training/learning cycles, and a large anisotropy in the fundamental control material parameter, in our case the electrical conductivity. In this work we report results on the improved performance of electrochemically controlled polymeric memristors, where optimization of a conducting polymer 共polyaniline兲 in the active channel and better environmental control of fabrication methods led to a large increase both in the absolute values of the conductivity in the partially oxydized state of polyaniline and of the on-off conductivity ratio. These improvements are crucial for the application of the organic memristor to adaptive complex signal handling networks. © 2009 American Institute of Physics.关DOI:10.1063/1.3153944兴
The memristor, a device which may be considered as a resistor with memory 共i.e., the resistance value depends on its previous history兲, was postulated many years ago,1
but only recently practical realizations have been reported. In particular, a recent work describes a completely inorganic nanoscale device in which the memory effect was explained by the dopant redistribution after the voltage application.2 However, a more reliable explanation of the memory effect may involve redox reactions in the active conduction medium.3
Redox reactions have been used as a working principle for several organic electronic devices. In particular, electro-chemical field-effect transistors have been extensively stud-ied for more than 20 years.4 The rectifying behavior ob-served for an electrochemical junction realized with a solid electrolyte5 can be considered as a further step toward the element with memory.
Some years ago we have reported a molecular electronic device, based on the electrochemical control of resistivity of a conducting polymer, which exhibited interesting electrical characteristics.6 Even if its construction seems to be rather similar to traditional electrochemical field-effect transistors, its working principle is actually closer to that of the electro-chemical rectifier.5 In particular, all conductivity variations occur in the restricted active area of a conducting polymer film in contact with a solid electrolyte. For this heterojunc-tion we have demonstrated several unusual electrical proper-ties, such as a memory effect of the device resistance,6which implies that it can be considered as a first example of a totally organic memristor, and current auto-oscillation
generation.7 Successive studies have indicated that the de-vice could be used as a main node in adaptive signal han-dling networks,8mimicking to some extent the learning be-havior of biological systems.9 Further development of this work for the realization of really complex networks capable of information processing and adaptive learning could open quite interesting perspectives. In particular, a critical feature of such systems would be the fact that the memory and in-formation processing functions would be performed by the same elements. Previous experience of the system will modify the properties of the constituting elements making it more adequate for the solving of new similar problems. Such behavior is the basis of synaptic learning, i.e., learning gov-erned by Hebbian rule.10 Similar processes are deemed to occur in biological organisms, where in many cases learning can be considered as the variation of the synaptic weight functions, which can vary the signal propagation pathways in the nervous system.11
The working principle of our device is based on the dif-ference in the conductivity of a conducting polymer, namely, polyaniline 共PANI兲 in the oxidized and reduced states.12 A detailed description of the device can be found in Ref.6. The device is schematically shown in Fig.1.
A thin PANI layer, used as a conducting channel, is
de-a兲Author to whom correspondence should be addressed. Tel.: ⫹39 0521 905235. FAX: ⫹39 0521 905223. Electronic mail: firstname.lastname@example.org.
FIG. 1. 共Color online兲 Schematic representation of the organic memristor with external power supply and measuring devices.
posited onto an insulating solid support with two metal elec-trodes. A stripe of solid electrolyte is deposited in the central part of the channel. The PANI area under the electrolyte is the active zone, as the oxidation and reduction in PANI take place in this area. Of course, some redox reactions can occur also outside this active zone due to possible diffusion. How-ever, the length of diffusion must be negligible with respect to the active zone width. In fact, micro-Raman investigation of the PANI state map as the device was cycled has demon-strated with micron resolution that all redox transformations take place within the active zone.13We expect, however, that the diffusion length is even significantly less than the reso-lution. The analysis of the kinetics of the conductivity trans-formations has shown that it requires about 20 min for arriv-ing to the saturation关diffusion to the whole PANI depth that is about 50 nm共Ref.6兲兴. Considering the working time val-ues in the present work, we can estimate the length as several nanometers that is really negligible with respect to the active zone width 共about 1 mm兲. A silver wire is attached to the electrolyte layer to be used as a reference point. In the nor-mal configuration the reference共gate兲 electrode is connected to the source and both of them are connected to the ground potential level. Thus, the reference potential is zero and re-duction or oxidation takes place according to the actual po-tential of the active zone. Even if the device is connected to the circuit by two points only, two different currents, namely, the ionic one in the electrolyte and the total current passing through the device, were measured and considered for better understanding of the device functioning. This by the way makes our device closer to the originally proposed memristor.1
The possibility of using such devices in adaptive net-works is determined by their property to increase their con-ductivity after application of a positive voltage higher than a certain value共usually +0.6 to +1.0 V depending on the par-ticular construction of the device兲 and its decrease after ap-plication of any negative voltage. The time constants of these variations are different: about one order of magnitude differ-ence in time constants necessary for saturating processes. Thus, unsupervised learning in the network will take place due to the increase in the conductivity of the elements lo-cated along pathways more frequently used for the signal transmission. Supervised learning, instead, will be performed by negative voltage application between input-output pairs connected by preferential pathways, formed during unsuper-vised learning of the system, but that are considered as a priori wrong. Such negative voltage application will inhibit the conductivity of elements along this pathway.
Simple circuits demonstrating the possibility of both supervised8and unsupervised9learning of networks based on these organic memristors have been already realized. How-ever, real complex共up to decision making兲 signal processing demands the formation of networks including a significantly larger number of such elements working for a rather long time共i.e., over thousands of learning cycles兲, necessary for effective learning. Thus, there are several requirements to memristor properties that must be satisfied before such net-works could be realized. First of all, the conductivity ratio in the oxidized conducting and reduced insulating states must
be as high as possible. In the previously realized elements there the ratio was about 100. Second, the absolute value of the conductivity of the memristor in the oxidized state must be rather high. In fact, if the signal pathways in the network contain thousands of such elements, high conductivity will guarantee a high signal-to-noise ratio level. Finally, it is very important to have high stability of the memristor properties. In the framework of the adaptive networks, the term “stabil-ity” has not the same meaning as for materials in traditional electronics, where it refers to the constant behavior of the functioning element in time. In our case instead the element must vary its electrical properties according to its previous history or due to the external training. Thus, we must con-sider some other parameter as an indication of the element stability. For this we consider the ability of the element to reproduce electrical properties’ variation during multiple cy-clic applications of variable potentials.
From this point of view we have already shown that the properties of the element realized on the basis of commer-cially available materials are rather stable for more than 4000 min and can allow at least 50 adaptations.14 Such stability permits the construction of networks capable to adaptations8 and mimicking learning of simple biological benchmarks;9 however, for complex signal processing, the stability must be increased.
The aim of this work is to investigate the influence of the channel composition and doping on the properties of the memristor with special emphasis on the three items de-scribed above, namely, conductivity ratio in reduced and dized states, absolute value of the conductivity in the oxi-dized state, and the stability of the device properties. For this last item, in particular, a new device configuration was de-veloped.
II. MATERIALS AND METHODS
Aniline共Aldrich, 99.5+% ACS 共American Chemical So-ciety specification of purity grade兲兲 was distilled under CaH2 at reduced pressure and stored in argon atmosphere. Dodecyl benzene sulfonic acid 共DBSA兲 共used for doping兲 共Fluka, 90% tech. isomers’ mixture兲, ammonium persulfate 共APS兲 共Fluka, 98% ACS 共American Chemical Society specification of purity grade兲, and N-methyl pyrrolidone 共1-methyl-2-pyrrolidinone, Aldrich, spectrophotometric grade, ⱖ99%兲 were used as received. Water HPLC共purity grade for High Performance Liquid Chromatography兲 grade was used.
PANI was prepared according to literature.15,16 Briefly, in a two-necked flask equipped with a mechanical stirrer and a dropping funnel, 14.40 g of DBSA dissolved in 800 ml of water and 4 g of aniline were gently added. The mixture was stirred for 3 h at room temperature until formation of the typical milklike solution of the anilinium salt and then the solution was cooled to 0 ° C by dipping the flask in a water-ice bath. Successively, five drops of a saturated solution of cobalt sulfate were added to the anilinium salt solution and then 10 g of APS dissolved in 35 ml of water were slowly dropped to the solution. After 5 h the stirring was stopped and the solution containing a blue-dark precipitate was stored for a night at room temperature. The precipitate was
collected by adding 1 l of methanol to the suspension and by filtering it with a Buchner filter. Finally the solid powder was repeatedly washed with methanol and water until neutrality. The PANI was then dried several days under vacuum pump. Infrared spectra 关Fourier transform infrared 共FTIR兲兴 were performed with a Fourier transform spectrometer “PerkinElmer™ Spectrum One” on films cast from N-methyl pyrrolidone solution on a KBr window. A list of the charac-teristic absorption bands studied is given as follows: FTIR 共cm−1兲: 3450 共N–H, NH 2−兲; 3236 共N–H兲; 2956 共asC–H, CH3−兲; 2924 共asC–H, CH2−兲; 2851 共sC–H, CH2−兲; 1557 共 N = Q = N兲; 1469 共N–B–N兲; 1384 共C–N, QBtQ兲; 1296 共 C–N, QBcQ, QBB, BBQ兲; 1233, 1256 共C–N, BBB兲; 1109 共␦ N = Q = N and Q = NH– Bo B – NH+– B兲; and 1032.
Elemental analyses共EAs兲 were accomplished by the mi-croanalysis laboratory at the Faculty of Pharmacy, University of Pisa.
EA共%, found兲: C 69.1; H 7.6; N 5.8; S 7.7.
Thermogravimetric scans were obtained with a Mettler Toledo Starc System moduloTGA/SDTA851eunder nitrogen flux, at a scan rate of 20 ° C/min.
TGA共°C, onset兲: 335.
UV-vis absorption spectra of polymer films were re-corded under isotropic conditions with a Perkin-Elmer Lambda 650 on films cast from N-methyl pyrrolidone solu-tion on quarts slide.
UV-vis共nm兲: 450, 800.
A special feature of such preparation is that the material is already partially doped before the beginning of the device construction.
Polyethylene oxide共8.000.000 Da兲 from Sigma with the concentration of 20 mg/ml doped with 0.1M LiClO4 was used as a solid electrolyte.
The active channel of the device was prepared by the deposition of 48 layers of PANI onto a glass substrate with two evaporated Cr electrodes, using the Langmuir–Schaefer 共horizontal dipping兲 technique. The multilayer was addition-ally doped by HCl treatment. Deposition and doping proce-dures were similar to those described in Ref.17.
About 1 mm in width stripe of Polyethylene oxide 共PEO兲 共 8.000.00 Da兲 was deposited in the central zone of the channel by solution casting. A 0.05 mm Ag wire was attached to the PEO stripe. The completed structure was ad-ditionally doped in HCl vapor.
An alternative “sandwich” structure for the device was tried. In this case the assembling procedure illustrated in Fig. 2 was as follows.
A PANI channel was formed on a glass support with two electrodes 共upper plate in Fig. 2兲 similarly to the previous case. A groove with a depth corresponding to the silver wire diameter was formed in the other solid support共glass兲. The
reference wire was placed into this groove and covered by a PEO solid electrolyte共bottom plate in Fig. 2兲. After drying for 30 min these two supports with formed structures were put in contact mechanically to form the device shown in Fig.2.
Electrical measurements were performed as follows: The source and gate electrodes were always at ground potential; the drain potential was swept between ⫺1.2 and +1.2 V, with steps of 0.1 V. Each sweep was started with a drain potential of 0 V, increasing it up to +1.2 V, then decreasing it until⫺1.2 V and finally increasing it back to 0 V. A 1 min delay was used after application of each voltage value and before the current reading, to allow the device to stabilize itself to the new conditions. Voltage sweep and drain current measurements were performed with a 236 source measure unit 共Keithley兲, while gate current measurements were per-formed with a 6514 system electrometer 共Keithley兲. Both Keithley units were linked to a PC and operated viaMATLAB
scripts, which allowed full automation of the measuring pro-cedure.
Initially, measurements were performed at ambient con-ditions. Measurements in a controlled environment were per-formed in a closed plastic chamber共about 1.5 l volume兲 with dried atmosphere and residual HCl vapor共about 10−4M, cor-responding to a partial pressure of about 200 Pa兲.
III. RESULTS AND DISCUSSION
The cyclic voltage-current characteristics of the device is shown in Fig. 3.
The characteristics show a pronounced rectifying behav-ior with hysteresis. In the initial stage of the cycle共low posi-tive potentials兲 the acposi-tive channel is in the insulating form. The transition to the conductive state takes place at the po-tential of about +0.6 V in good agreement with our previous measurements when PANI was doped only with HCl.6In the back scan of the voltage the device has high conductivity with practically Ohmic behavior. Its transition to the insulat-ing state takes place at about 0.1 V of the drain voltage.
From the behavior of the characteristics we can conclude that the two critical requirements for the memristor electrical properties, mentioned in the Introduction, are satisfied. In fact, the device has very high conductivity in the conductive
FIG. 2. 共Color online兲 Scheme of the element with sandwich structure.
-20.00 0.00 20.00 40.00 60.00 80.00 -1.5 -1 -0.5 0 0.5 1 1.5 Voltage (V) Cu rr en t(µ A)
FIG. 3. Cyclic voltage-current characteristics of the organic memristor. The arrows indicate the direction共increase or decrease兲 of the voltage scan.
state. The reached current value is more than 60 A 共at a voltage of 1.0 V兲, which is much higher with respect to our previous results 共1.0–2.0 A兲; furthermore, the conductiv-ity ratio of the device in the conducting and insulating states, which is probably even more important for the realization of the adaptive networks, jumped from about 100 for the posi-tive and negaposi-tive branches of the cyclic voltage-current char-acteristics to about 2000 in the present device. This improve-ment of more than one order of magnitude is a very encouraging result. The kinetics of the conductivity variation is also an important characteristic of the device. The tempo-ral behavior of the ionic 共gate兲 and electron 共drain minus gate兲 currents through the device for positive and negative potentials is shown in Fig.4.
From a comparison with our previous results6 we see that the time constant of the conductivity variation in the case of the negative potential is similar, while for the positive voltage it becomes faster. This last finding can be due to the increased conductivity ratio for two different states of the PANI channel. In fact, the slower kinetics for the positive potential was explained by the gradual oxidation of the PANI in the active zone and continuous spatial redistribution of the potential along its length. If the conductivity anisotropy is increased, such redistribution should occur faster. In order to check this hypothesis we have applied the model18that was successfully used to interpret not only differences in the con-ductivity variation kinetics for negative and positive polari-ties but also the appearance of auto-oscillations of the current for the device capable for the charge accumulation.7Within the model, the active zone is divided in narrow stripes with its own timer. Conductivity variations take place within each stripe after passing reduction or oxidation potential with re-spect to the reference electrode according to the kinetics, experimentally found for the negative bias. The program re-calculates electronic and ionic currents, and voltage distribu-tion profile along the PANI channel after each time intervals. The results of the simulations are shown in Fig. 5 for the device with standard properties 共b兲 and with those observed in the present case共a兲, i.e., increased difference in conduc-tivities for oxidized and reduced states and with increased ionic conductivity.
However, multicycle investigation of the device proper-ties has revealed that the stability of the electrical properproper-ties was similar to those for the element with a standard channel.14 The degradation of the properties was attributed previously to the partial dedoping of the PANI layer. There-fore, further measurements were performed in the chamber with controlled HCl partial pressure. The temporal behavior of the drain current during the application of cyclic scans of the drain voltage is shown in Fig. 6.
Logarithmic dependence of the peak current value on the number of cycle is shown in Fig.7. The absolute value of the device conductivity decreases exponentially for the first 5 cycles and then becomes practically constant after the tenth cycle, remaining still very high with respect to even freshly prepared samples measured in the ambient conditions. The initial decrease in the conductivity is a normal phenomenon for the conducting polymers, which can be due to several factors, such as some contact processes on the boundary with metal electrodes or redistribution of the dopant upon reach-ing equilibrium conditions. Thus, the conditions with re-sidual acid vapor can improve the performance of the device. -8.00 -6.00 -4.00 -2.00 0.00 2.00 4.00 6.00 0 1000 2000 3000 4000 Time (s) C ur re nt (µ A) ionic current electron current
FIG. 4. Temporal behavior of the electron and ionic currents of the organic memristor for positive共+0.6 V; point A兲 and negative 共⫺0.2 V, point B兲 drain voltages. 0 2000 4000 6000 8000 10000 12000 0.0 1.0x10-6 2.0x10-6 3.0x10-6 4.0x10-6 5.0x10-6 6.0x10-6 b a Time (sec) C urrent (A )
FIG. 5. Simulations of the conductivity variation for the device biased with +0.6 V according to the model described in Ref.10.共a兲 Device with in-creased difference of the conductivity in oxidized and reduced states共two orders of magnitude higher than in previous case兲 and with increased ionic conductivity 共one order of magnitude higher than in previous case兲. 共b兲 Device with previously共Ref.2兲 described properties.
-10.00 0.00 10.00 20.00 30.00 40.00 50.00 0 40000 80000 120000 160000 200000 Time (s) C ur re n t (µ A )
FIG. 6. Temporal behavior of the drain current during multicycle applica-tion of the drain voltage.
However, an element that does not demand the use of special measuring chambers would be more practical. A solution could be to prevent dedoping by appropriate sealing. The first step in this direction was performed by assembling the device in a sandwich configuration共Fig.2兲. Confinement of the active zone between two solid plates was expected to make more difficult the dedoping of PANI. The results of the drain current temporal behavior during multicyclic applica-tion of the drain voltage were found to be similar to those obtained in controlled conditions共Fig.6兲. We have observed the rather significant decrease in the maximum drain current for first cycles. However, after 5 cycles, the characteristics were well stabilized. Cyclic voltage-current characteristics for cycles 6–8 are shown in Fig.8.
As it is clear from Fig.8, such sealing has resulted in the significant improvement of the device properties’ stability, which persisted for many successive cycles.
Utilization of PANI, predoped with a rather strong acid 共DBSA兲, resulted in the improvement of two important pa-rameters of the polymeric electrochemical device 共organic memristor兲, namely, the conductivity ratio in conducting and insulating states and in the absolute value of the conductivity for the positive polarity of the applied voltage. Due to the presence of the high molecular weight anion, the use of DBSA during the PANI synthesis guarantees the significant decrease in the dedoping rate, which is rather high in the case of HCl doping, resulting in the improvement of the device characteristics and its working time. This result is very im-portant for the successful realization of the adaptive net-works based on a large number of such elements. We can expect, in fact, a high signal-to-noise ratio and possibility of effective supervised and unsupervised learning of the system. The increase in the stability of electrical properties’ variation can be obtained by measurements in controlled conditions or by effective sealing of the fabricated structures.
We acknowledge the financial support of the Future and Emerging Technologies 共FET兲 programme within the Sev-enth Framework Programme for Research of the European Commission, under the FET-OPEN grant agreement BION, Grant No. 213219.
1L. O. Chua,IEEE Trans. Circuit Theory18, 507共1971兲.
2D. B. Strukov, G. S. Snider, D. R. Stewart, and R. S. Williams,Nature
3J. Wu and R. L. McCreery,J. Electrochem. Soc.156共1兲, P29 共2009兲. 4C. F. Shu and M. S. Wrighton,J. Phys. Chem.92, 5221共1988兲. 5M. Chen, D. Nilsson, T. Kugler, and M. Berggren,Appl. Phys. Lett.81,
6V. Erokhin, T. Berzina, and M. P. Fontana,J. Appl. Phys. 97, 064501 共2005兲.
7V. Erokhin, T. Berzina, P. Camorani, and M. P. Fontana,J. Phys.: Condens.
8V. Erokhin, T. Berzina, and M. P. Fontana, Crystallogr. Rep. 52, 159 共2007兲.
9A. Smerieri, T. Berzina, V. Erokhin, and M. P. Fontana,Mater. Sci. Eng.,
10D. O. Hebb, The Organization of Behavior: A Neuropsychological Theory, 2nd ed.共Wiley, New York, 1961兲.
11P. R. Benjamin, K. Staras, and G. Kemenes,Learn. Memory7, 124共2000兲. 12E. T. Kang, K. G. Neoh, and K. L. Tan,Prog. Polym. Sci.23, 277共1998兲. 13T. Berzina, V. Erokhin, and M. P. Fontana,J. Appl. Phys. 101, 024501
14V. Erokhin, T. Berzina, P. Camorani, and M. P. Fontana,Colloids Surf., A
15Y. Haba, E. Segal, M. Narkis, G. I. Titelman, and A. Siegmann,Synth.
16W. A. Gazotti and M.-A. De Paoli,Synth. Met.80, 263共1996兲. 17V. I. Troitsky, T. S. Berzina, and M. P. Fontana,Synth. Met. 129, 39
18A. Smerieri, V. Erokhin, and M. P. Fontana,J. Appl. Phys.103, 094517 共2008兲.
1 10 100
0 5 10 15 20
Number of the cycle
FIG. 7. Logarithmic dependence of the peak current on the number of the cycle. -1.0 -0.5 0.0 0.5 1.0 0.0 5.0x10-7 1.0x10-6 1.5x10-6 2.0x10-6 2.5x10-6 3.0x10-6 Curr ent (A) Voltage (V)
FIG. 8. Cyclic voltage-current characteristics for a sandwich structure for the fifth, sixth, and seventh cycles. The arrows indicate the direction 共in-crease or de共in-crease兲 of the voltage scan.